Removal of 10-nm contaminant particles from Si wafers using CO2 bullet particles
© Kim et al; licensee Springer. 2012
Received: 25 October 2011
Accepted: 11 April 2012
Published: 11 April 2012
Removal of nanometer-sized contaminant particles (CPs) from substrates is essential in successful fabrication of nanoscale devices. The particle beam technique that uses nanometer-sized bullet particles (BPs) moving at supersonic velocity was improved by operating it at room temperature to achieve higher velocity and size uniformity of BPs and was successfully used to remove CPs as small as 10 nm. CO2 BPs were generated by gas-phase nucleation and growth in a supersonic nozzle; appropriate size and velocity of the BPs were obtained by optimizing the nozzle contours and CO2/He mixture fraction. Cleaning efficiency greater than 95% was attained. BP velocity was the most important parameter affecting removal of CPs in the 10-nm size range. Compared to cryogenic Ar or N2 particles, CO2 BPs were more uniform in size and had higher velocity and, therefore, cleaned CPs more effectively.
KeywordsNano-bullet CO2 Supersonic nozzle Gas-phase nucleation Cleaning efficiency
The manufacturing yield of submicron-scale devices can be reduced by particulate contamination of their surfaces. Sizes of semiconductor device features are expected to decrease continuously, reaching 25 nm by 2015 for DRAM/flash memory devices, and together with this decrease, critical killer particle size is expected to decrease to 12.5 nm . In the nanometer range, the adhesion force per contact area between a particle and surface increases linearly as particle size decreases, but the fluid drag force changes in proportion to the cross-sectional area of a particle  so the use of drag force to remove contaminant particles (CPs) becomes less efficient as CP size decreases [3–6].
One promising method of removing very small CPs is the cryogenic aerosol technique in which the contaminated surface is bombarded by fine, high-velocity bullet particles (BPs) made of volatile material. CPs on the surface can be removed if the energy transferred from BPs to the CP is sufficient to overcome the adhesion energy between the CP and the substrate [7, 8]. In the conventional form of this technology, condensable gas is pre-cooled close to liquid nitrogen temperature and, then, expanded through a simple nozzle such as a cylindrical hole. Cooling liquefies some of the condensable gas; expansion of the gas through the nozzle atomizes the liquid into fine droplets, and adiabatic cooling causes solid particles to form during further expansion. Typical particle size is a few microns, and typical velocity is 100 m/s. The minimum size of CP that can be removed efficiently using these micron-sized particles is approximately 50 nm [6–10].
Simulations suggest that reducing the size of the BP and projecting it at higher velocity can increase the effectiveness of CP removal even if the kinetic energy of the BPs is not changed . If the BP is too big compared to the target CP, the atoms or molecules released by the BP when it fragments after collision with the CPs or the substrate may prevent the CP from leaving the surface ; this implies that BPs must be less than some maximum size if they are to effectively remove nanometer-size CPs. A new particle beam technique using Ar BPs has been developed and used to remove CPs of 20-nm size from flat surfaces and trenches [12, 13]; its success was attributed to the nanometer size and supersonic velocity of the BPs.
Despite the success, two practical difficulties using Ar BPs remain: (1) BP size is very sensitive to temperature , so it must be controlled very accurately to achieve size uniformity, and (2) BP velocity is limited by low temperature. Generating BPs at room temperature (RT) would eliminate the need to control temperature and increase BP velocity. The resulting uniform, fast BPs should improve removal of nanometer CPs.
The aim of this study is, thus, to explore the possibility of extending the capability of the nanoparticle beam technique down to 10-nm size by increasing BP velocity. Adhesion force per contact area for a 10-nm particle is twice as high as that for a 20-nm particle, so an appropriate combination of size and velocity of the BPs is needed to overcome this high adhesion force. Pure CO2 or a mixture of CO2 and He was used to generate nano-sized CO2 BPs with supersonic velocity. This technique is unique in that nano-sized CO2 BPs are used and that 10-nm CPs are removed.
To generate BPs traveling at the greatest possible supersonic velocity, pure CO2 or CO2/He mixture gas was used. Stagnation pressure was varied in the range of 5-50 bar; stagnation temperature was kept at RT. The shape and size of the nozzle were adjusted to make the Mach number at the nozzle exit > 5.0 over the whole range of experimental conditions. The nozzle is nearly conical at the throat but rapidly expands near the exit to compensate for boundary layer growth and to prevent shock wave formation.
In all trials, the CPs were 10-nm Al2O3 particles (Aldrich No. 642991, Sigma-Aldrich Corporation, St. Louis, MO, USA); they were generated by spin coating a drop of Al2O3 solution onto a wafer which was then dried for a few days in dry N2 gas. Based on the nucleation rate predicted by a classical nucleation theory and measured particle velocity, the rate of bombardment by the BPs is estimated at about 1,000-10,000/s on every square of 20-nm side . Thus, cleaning was completed within 1-2 s of exposure in all the cases shown. The cleaning was unprecedentedly fast which is attributed to the extremely high rate of nuclei formation during homogeneous nucleation under highly supersaturated conditions. Evaporation of CO2 BPs after collision on the wafer surface generates a gas flow of high velocity which is strong enough to carry the dislodged CPs to the vent exit.
Scanning electron microscope (SEM) images were taken before and after cleaning. The cleaning efficiency was determined by the change in the surface area covered by the CPs, and the removal area was measured using the Image J, a free software distributed by the US National Institute of Health (MD, USA). Nozzle-wafer distance and the angle of the particle beam incident on the wafer varied, but the photographs shown were all taken when the incident angle of the particle beam was 30° to the normal. Chamber pressure was maintained low enough to ensure supersonic flow inside the nozzle.
Results and discussion
Therefore, a CO2/He mixture gas was used to increase BP velocity. Because supersonic flow speed varies with specific-heat ratio (R) and molecular weight (M) of the gas as approximately (R/M)1/2, the use of light carrier gas with high R like He is expected to give very high BP velocity. According to inviscid flow theory, expected velocity increase over pure CO2 is approximately 45% for a 1:1 CO2/He mixture, 120% for a 1:4 mixture and 180% for a 1:9 mixture, but measured increase in velocity with mixture fraction was much smaller than expected, i.e., 5%, 30%, and 50% for 1:1, 1:4, and 1:9 CO2/He mixtures, respectively (Figure 6); this difference can be attributed again to the increased boundary layer thickness due to the highly viscous He gas.
The consistent increase in removal efficiency with He fraction at the same BP size implies that BP velocity has the greatest effect on the removal of nanometer-sized CPs. BP size is important only in that the BP must be big enough to have total kinetic energy sufficiently higher than the CP-surface adhesion energy, but at the same time smaller than a critical size at which dispersal of removed CPs is inhibited by the atoms or molecules emitted during breakup of the BP. If the useful BP size is on the same order as the target particle as was observed in this study, using BPs that are smaller than the conventional micron particles by a factor of about 100 is expected to damage the substrate much less than micron particles because damage is proportional to the total kinetic energy of each BP.
The feasibility of removing 10-nm CPs from a substrate using nano-sized volatile BPs was proven experimentally: (1) by controlling the nozzle contour and expansion pressure, CO2 particles of 5-50-nm size were generated by gas-phase nucleation and growth; (2) when using a carrier gas mixture of 1:9 CO2/He, the particle beam generated in this study could remove 10-nm CPs with efficiency > 95%; (3) the velocity of the BPs was the most important factor in determining the effectiveness of CP removal, and the use of light carrier gas (He) was effective in increasing flow velocity; (4) cleaning effectiveness increased with decrease in chamber pressure; and (5) compared to Ar or N2 particles generated by liquid atomization, CO2 BPs were more uniform in size and had higher velocity and, therefore, cleaned CPs more effectively.
Atomic force microscope
Scanning electron microscope.
This work was supported by the Korea Research Foundation (KRF) grant funded by the Korean government (MOE) (grant no. ROA-2008-000-20045-0).
- SEMATECH and International Technology Roadmap for Semiconductors: 2009 Yield enhancement report and table.[http://www.itrs.net/Links/2009ITRS/Home2009.htm]
- Rimai DS, Quesnel DJ: Fundamentals of Particle Adhesion. CA, USA: Global Press; 2001.
- Sherman R: Carbon dioxide snow cleaning. In Particles on Surfaces 5 & 6: Detection, Adhesion and Removal. Edited by: Mittal KL. Netherlands: VSP; 1999:221–237.
- Bakhtari K, Guldiken RO, Makaram P, Busnaina AA, Park JG: Experimental and numerical investigation of nanoparticle removal using acoustic streaming and the effect of time. J Electrochem Soc 2006, 153: G846-G850. 10.1149/1.2217287View Article
- Lim H, Jang D, Kim D, Lee JW, Lee J: Correlation between particle removal and shock-wave dynamics in the laser shock cleaning process. J Applied Phys 2005, 97: 054903–054908. 10.1063/1.1857056View Article
- Lin H, Chioujones K, Lauerhaas J, Freebern T, Yu C: Damage-free cryogenic aerosol clean processes. J IEEE Trans Semicond Manuf 2007, 20: 101–106.View Article
- McDermott WT, Ockovic RC, Wu JJ, Miller RJ: Removing submicron surface particles using a cryogenic argon-aerosol technique. J Microcontamination 1991, 9: 33–36.
- McDermott WT, Sferlazzo P: Argon aerosol surface cleaning: an overview. In Particles on Surfaces 5 & 6: Detection, Adhesion and Removal. Edited by: Mittal KL. Netherlands: VSP; 1999:239–249.
- Lauerhaas JM, Weygand JF, Thomes GP: Advanced cryogenic aerosol cleaning: application to damage-free cleaning of sensitive structured wafers. In IEEE/SEMI Advanced Semiconductor Manufacturing Conference: 2005 April 11–12; Munich. MN, USA: FSI; 2005:11.View Article
- Wagener TJ, Kawaguchi K: Improved yields for the nano-technology era using cryogenic aerosols. In IEEE/SEMI Advanced Semiconductor manufacturing Conference: 2004 May 4–6; Boston. MN, USA: FSI; 2004:467.
- Yi M, Kim D, Lee JW, Koplik J: Molecular dynamics (MD) simulation on the collision of a nano-sized particle onto another nano-sized particle adhered on a flat substrate. J Aerosol Sci 2005, 36: 1427–1443. 10.1016/j.jaerosci.2005.03.013View Article
- Lee JW, Kang K, Lee K, Yi M, Lee M: Removing 20 nm particles using a supersonic argon particle beam generated with a contoured Laval nozzle. J Adhesion Sci Tech 2009, 23: 769–777. 10.1163/156856108X396264View Article
- Hwang K, Lee K, Yi M, Lee JW: Removing 20 nm ceramic particles using a supersonic particle beam from a contoured Laval nozzle. J Thin Solid Films 2009, 517: 3866–3869. 10.1016/j.tsf.2009.01.132View Article
- Bae H, Kim I, Kim E, Lee JW: Generation of nano-sized Ar-N2 compound particles by homogeneous nucleation and heterogeneous growth in a supersonic expansion. J Aerosol Science 2010, 41: 243–256. 10.1016/j.jaerosci.2009.11.005View Article
- Becker R, Doering W: Kinetische behandlung der keimbildung in übersättigten dämpfen. J Ann Phys 1935, 24: 719–752.View Article
- Hill PG: Condensation of water vapour during supersonic expansion in nozzles. J Fluid Mechanics 2006, 25: 593–620.View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.